CHAPTER 7: MECHANICAL PROPERTIES

Presentation on theme: "CHAPTER 7: MECHANICAL PROPERTIES"— Presentation transcript:

CHAPTER 7: MECHANICAL PROPERTIES
ISSUES TO ADDRESS... • Stress and strain: What are they and why are they used instead of load and deformation? • Elastic behavior: When loads are small, how much deformation occurs? What materials deform least? • Plastic behavior: At what point do dislocations cause permanent deformation? What materials are most resistant to permanent deformation? • Toughness and ductility: What are they and how do we measure them? Ceramic Materials: What special provisions/tests are made for ceramic materials? 1

Elastic means reversible! 2

PLASTIC DEFORMATION (METALS)

ENGINEERING STRESS • Tensile stress, s: • Shear stress, t:
Stress has units: N/m2 or lb/in2 4

COMMON STATES OF STRESS
• Simple tension: cable Ski lift (photo courtesy P.M. Anderson) • Simple shear: drive shaft Note: t = M/AcR here. 5

OTHER COMMON STRESS STATES (1)
• Simple compression: (photo courtesy P.M. Anderson) Note: compressive structure member (s < 0 here). (photo courtesy P.M. Anderson) 6

OTHER COMMON STRESS STATES (2)
• Bi-axial tension: • Hydrostatic compression: Pressurized tank (photo courtesy P.M. Anderson) (photo courtesy P.M. Anderson) s < 0 h 7

ENGINEERING STRAIN • Tensile strain: • Lateral strain: • Shear strain:
Strain is always dimensionless. 8

STRESS-STRAIN TESTING
• Typical tensile specimen • Typical tensile test machine Adapted from Fig. 6.2, Callister 6e. • Other types of tests: --compression: brittle materials (e.g., concrete) --torsion: cylindrical tubes, shafts. Adapted from Fig. 6.3, Callister 6e. (Fig. 6.3 is taken from H.W. Hayden, W.G. Moffatt, and J. Wulff, The Structure and Properties of Materials, Vol. III, Mechanical Behavior, p. 2, John Wiley and Sons, New York, 1965.) 9

LINEAR ELASTIC PROPERTIES
• Modulus of Elasticity, E: (also known as Young's modulus) • Hooke's Law: s = E e • Poisson's ratio, n: metals: n ~ 0.33 ceramics: ~0.25 polymers: ~0.40 Units: E: [GPa] or [psi] n: dimensionless 10

PROPERTIES FROM BONDING: E
• Elastic modulus, E • E ~ curvature at ro E is larger if Eo is larger. 11

OTHER ELASTIC PROPERTIES
• Elastic Shear modulus, G: simple torsion test t = G g • Elastic Bulk modulus, K: pressure test: Init. vol =Vo. Vol chg. = DV • Special relations for isotropic materials: 12

YOUNG’S MODULI: COMPARISON
Graphite Ceramics Semicond Metals Alloys Composites /fibers Polymers E(GPa) Based on data in Table B2, Callister 6e. Composite data based on reinforced epoxy with 60 vol% of aligned carbon (CFRE), aramid (AFRE), or glass (GFRE) fibers. 13

USEFUL LINEAR ELASTIC RELATIONS
• Simple tension: • Simple torsion: • Material, geometric, and loading parameters all contribute to deflection. • Larger elastic moduli minimize elastic deflection. 14

PLASTIC (PERMANENT) DEFORMATION
(at lower temperatures, T < Tmelt/3) • Simple tension test: 15

YIELD STRENGTH, sy • Stress at which noticeable plastic deformation has occurred. when ep = 0.002 16

YIELD STRENGTH: COMPARISON
Room T values Based on data in Table B4, Callister 6e. a = annealed hr = hot rolled ag = aged cd = cold drawn cw = cold worked qt = quenched & tempered 17

TENSILE STRENGTH, TS • Maximum possible engineering stress in tension.
Adapted from Fig. 6.11, Callister 6e. • Metals: occurs when noticeable necking starts. • Ceramics: occurs when crack propagation starts. • Polymers: occurs when polymer backbones are aligned and about to break. 18

TENSILE STRENGTH: COMPARISON
Room T values Based on data in Table B4, Callister 6e. a = annealed hr = hot rolled ag = aged cd = cold drawn cw = cold worked qt = quenched & tempered AFRE, GFRE, & CFRE = aramid, glass, & carbon fiber-reinforced epoxy composites, with 60 vol% fibers. 19

DUCTILITY, %EL • Plastic tensile strain at failure:
Adapted from Fig. 6.13, Callister 6e. • Another ductility measure: • Note: %AR and %EL are often comparable. --Reason: crystal slip does not change material volume. --%AR > %EL possible if internal voids form in neck. 20

TOUGHNESS • Energy to break a unit volume of material
• Approximate by the area under the stress-strain curve. 21

HARDENING • An increase in sy due to plastic deformation.
• Curve fit to the stress-strain response: 22

MEASURING ELASTIC MODULUS
• Room T behavior is usually elastic, with brittle failure. • 3-Point Bend Testing often used. --tensile tests are difficult for brittle materials. Adapted from Fig , Callister 6e. • Determine elastic modulus according to: 23

MEASURING STRENGTH • 3-point bend test to measure room T strength.
Adapted from Fig , Callister 6e. • Flexural strength: • Typ. values: Si nitride Si carbide Al oxide glass (soda) 69 300 430 390 69 Data from Table 12.5, Callister 6e. 24

TENSILE RESPONSE: ELASTOMER CASE
Stress-strain curves adapted from Fig. 15.1, Callister 6e. Inset figures along elastomer curve (green) adapted from Fig , Callister 6e. (Fig is from Z.D. Jastrzebski, The Nature and Properties of Engineering Materials, 3rd ed., John Wiley and Sons, 1987.) • Compare to responses of other polymers: --brittle response (aligned, cross linked & networked case) --plastic response (semi-crystalline case) 25

T AND STRAIN RATE: THERMOPLASTICS
• Decreasing T... --increases E --increases TS --decreases %EL • Increasing strain rate... --same effects as decreasing T. Adapted from Fig. 15.3, Callister 6e. (Fig is from T.S. Carswell and J.K. Nason, 'Effect of Environmental Conditions on the Mechanical Properties of Organic Plastics", Symposium on Plastics, American Society for Testing and Materials, Philadelphia, PA, 1944.) 26

TIME DEPENDENT DEFORMATION
• Stress relaxation test: • Data: Large drop in Er for T > Tg. (amorphous polystyrene) --strain to eo and hold. --observe decrease in stress with time. Adapted from Fig. 15.7, Callister 6e. (Fig is from A.V. Tobolsky, Properties and Structures of Polymers, John Wiley and Sons, Inc., 1960.) • Relaxation modulus: • Sample Tg(C) values: PE (low Mw) PE (high Mw) PVC PS PC -110 - 90 + 87 +100 +150 Selected values from Table 15.2, Callister 6e. 27

HARDNESS • Resistance to permanently indenting the surface.
• Large hardness means: --resistance to plastic deformation or cracking in compression. --better wear properties. Adapted from Fig. 6.18, Callister 6e. (Fig is adapted from G.F. Kinney, Engineering Properties and Applications of Plastics, p. 202, John Wiley and Sons, 1957.) 28

DESIGN OR SAFETY FACTORS
• Design uncertainties mean we do not push the limit. • Factor of safety, N Often N is between 1.2 and 4 • Ex: Calculate a diameter, d, to ensure that yield does not occur in the 1045 carbon steel rod below. Use a factor of safety of 5. 5 29

SUMMARY • Stress and strain: These are size-independent
measures of load and displacement, respectively. • Elastic behavior: This reversible behavior often shows a linear relation between stress and strain. To minimize deformation, select a material with a large elastic modulus (E or G). • Plastic behavior: This permanent deformation behavior occurs when the tensile (or compressive) uniaxial stress reaches sy. • Toughness: The energy needed to break a unit volume of material. • Ductility: The plastic strain at failure. Note: For materials selection cases related to mechanical behavior, see slides 20-4 to 30

ANNOUNCEMENTS Reading: Core Problems: Self-help Problems: